Presentation on theme: "Tsnl Synthesis and Application of Nanosize Semiconductors for Photoxidation of Toxic Organic Chemicals Acknowledgement: Div. Of Materials Science and Engineering,"— Presentation transcript:
tsnl Synthesis and Application of Nanosize Semiconductors for Photoxidation of Toxic Organic Chemicals Acknowledgement: Div. Of Materials Science and Engineering, Office of Science, US Dept. of Energy under contract DE-AC-04-AL8500. Sandia is a multiprogram laboratory operated by Sandia Corporation, a Lockheed-Martin Company, for the US Dept. of Energy. This work performed under the aupices of the DOE Environmental Science/Environmental Research (ER/ES) Program. Industrial Solvents in the Environment (Impregnated Sediments, Water Table) Brief History of the problem and possible remediation approaches (Bioremediation, Soil Washing, Adsorption, Photooxidation) Photocatalysis using UV light and nanosize TiO 2 and SnO 2. Photocatalysis using visible light and MoS 2 nanoclusters. J.P. Wilcoxon, Nanostructures and Advanced Materials Chemistry Sandia National Laboratories Albuquerque, N.M., Colloborators: T.R. Thurston, P. Provencio, G.A. Samara Talk Outline
tsnl Typical Scenario-Dense Non-Aqueous Solvent Pools Examples- Cleaning Solvents- Tri-Chloroethylene (TCE) Herbicides/Fungacides/Pesticides (Pentachlorophenol (PCP), DDT) Explosives (e.g. TNT) Major Remediation Issues- 1) Low Solubility (1-10 ppm) in water provides continuous leaching with time 2) Treatment of large volumes of highly diluted toxins 3) Cost of treatment Rain Organic Pool in Soil Water Table Slow Leaching
tsnl Possible Treatment Approaches- Conventional Treatment Options: 1)Filtration and/or Adsorption of toxic chemicals in aqueous supernatant from Step 1 2)Chemical Oxidation or Total Mineralization of the the Organics 3)Deep UV Photooxidation of the Organics 4)Photocatalytic oxidation of the Organics (e.g. colloidal titania slurries) Step 1: Excavation, Soil Washing Cost and large volumes involved are the principal practical concerns.
tsnl Alternative Approach Use stable, inorganic, semiconductor nanoclusters with tunable bandgaps to oxidize organic chemicals using sunlight Clusters can be used in both dispersed and heterogeneous forms (supported) MoS 2 nanocrystal + + electron/hole transfer reactions CO 2 + HCl sunlight - - chlorinated aromatic + H 2 O e h +
tsnl Advantanges of this Approach- The light absorption and energy levels of the semiconductor valence and conduction bands can be adjusted in a single material by changing the size (quantum confinement effect). A covalent semiconductor material with excellent photostability and low toxicity can be selected (e.g. MoS 2 ). Our synthesis allows easy chemical modification of the nanocluster surface properties (e.g. deposition of a metal). Small size of nanocluster vastly reduces electron-hole recombination rate and undesired light scattering. Nanoclusters are easily deposited on bulk support materials from a dispersed liquid phase. Both dispersed and supported nanoclusters can be studied, allowing complete characterization of the photocatalyst microstructure.
tsnl Photocatalysts Material Requirements - 1) Efficient conversion of sunlight to electron-hole pairs. 2) Surface trapping of electrons and holes before recombination. 3) Catalyst photostability. 4) Inexpensive, chemically-stable, environmentally benign materials.
tsnl MoS 2 layered structure gives chemical stability- Binding of substrate organic chemical occurs at metal edge sites. Electron transfer rates allow an estimation of shift of the redox potential with size
tsnl MoS 2, Like TiO 2 Has Exceptional Photostability- Kinetic stability occurs because both valence and conduction bands are localized on the metal, so carrier excitation doesn’t weaken any chemical bonds Energy Valence Band S 3p MoS 2 Mo, 4 d z 1.33 V Conduction Band Mo, 4d xy 0.1 V light S 3p CdS Cd, 5s V Covalent Semi-conductors (Stable) Ionic II-VI Materials Carrier Excitation Weakens Chemical Bonds (Unstable)
tsnl MoS 2 synthesis, purification, and characterization- Synthesis in Inverse Micelle System Mo S 2- = MoS 2 Mo Source: MoCl 4, S Source: H 2 S, Oil: Octane Typical Surfactant: Tri-ocytlmethylammonium Chloride (TOAC)
tsnl Purification by extraction into Acetonitrile (ACN) 1) Liquid Chromatography shows the MoS 2 clusters have a net charge. 2) Samples diluted into water are dialized to remove unwanted ions like SO ) Analysis by XRF gives the final [Mo] and [Mo]:[S]~ 1 : 2.4 for D=3 nm. MoS2 In Oil ACN With hydrophilic cationic Surfactant With Hydrophobic TOAC Surfactant Oil MoS2 In ACN
tsnl Quantum Size Effects influence the optical and electronic properties of the resulting solutions- By adjusting the size alone, the conductance and valence band energy levels can be shifted allowing new types of photocatalytic behavior to occur
tsnl Structural/Size Characterization- Chromatogram of clusters Linewidth(polydispersity) comparable to chemical impurities
tsnl Light Absorbance and Redox Potentials- Greater light absorbance reduces the ability to oxidize a given organic. n Mixtures of Nanoclusters will likely optimize the photooxidation process.
tsnl Photochemical Reactor- 400 W Xe arc lamp with long pass filters. n Cylindrical reactor with sampling port and overhead illumination.
tsnl Liquid Chromatography is Used to Follow the Kinetics of Photo-Redox Reactions- Basic Concept - Chemicals (and dispersed nanoclusters) travel through a porous medium which separates them and they elute at various times. The amount of chemical in each elution peak is measured using an absorbance or fluorescence detector and compared to known amounts of the same chemical. Intermediate break-down products are also identified. The size of the elution peak at a chosen absorbance wavelength gives the amount of each chemical. The stability of the nanosize photocatalyst can be determined from changes in the complete absorbance spectrum at its elution peak Absorbance (250 nm) elution time (min) MoS 2 Photocatalyst t = 0 organic impurity increasing time Organic Impurity Oxidized to CO 2 Example - Destruction of an Alkyl Chloride Organic Impurity using dispersed nanosize (D = 3 nm) MoS 2.
tsnl Optical Absorbance of Nanocluster Catalyst is Unchanged- No reduction in optical absorbance, nanocluster concentration, or photocatalytic activity were observed
tsnl Photocatalysis of Phenol Using Nanosize MoS 2 Supported on TiO 2 Powder Visible Light Absorbance by MoS 2. Carrier transfer between MoS 2 and TiO 2 slurry particles decreases recombination rate and increases photooxidation rate of organic.
tsnl Photocatalysis of Phenol Using Nanosize MoS 2 Supported on TiO 2 Powder Visible ( >450 nm)Light Absorbance by MoS 2 shows exponential photo-oxidation kinetics. A strong size dependence of photo-oxidation rate is observed.
tsnl Pentachlorophenol (PCP) Photocatalysis Studies- Intermediate Photooxidation Products Depend on Catalyst Material UV Photooxidaton using D=25 nm, SnO 2 Clusters PCP UV Photooxidation Results using TiO 2 (Degussa)
tsnl PCP Photooxidation Results(Summary) CO 2 measured at end of reaction confirms total photooxidation of PCP. Visible Light Photooxidation Results PCP UV Photooxidation Results
tsnl Conclusions Photo-oxidation of an alkyl chloride by nanosize MoS 2 shows a strong size dependence and occurs with weak visible illumination. HPLC analysis demonstrates that no changes occur in the quantity or absorbance properties of nanosize MoS 2 during the photooxidation of this alkyl chloride. Both nanosize SnO 2 and MoS 2 show a strong size-dependent photocatalytic activity. Nanosize MoS 2 can be an effective photocatalyst for PCP photo- oxidation even with only visible ( >400 nm) light.
tsnl Future Directions Improve nanocluster/support interactions by heat treatments after deposition of nanoclusters to improve photocatalysis kinetics. Examine nanocluster systems with mixed sizes (bandedges and potentials) to optimize solar absorbance while still allowing a sufficient driving force for the photooxidation process. Examine the photooxidation of long-lived organics such as pesticides, and polycyclic aromatics using nanosize MoS 2 to determine reaction kinetics and final breakdown products. Investigate alternative, highly stable nanocluster catalysts (RuS 2, WS 2 ) and compare with MoS 2. Investigate other small molecule photoredox reactions (e.g. H 2 O or H 2 S reduction.